Covalent superconductor

Superconducting materials where the atoms are linked by covalent bonds

Parts of a high pressure cell after the synthesis of heavily boron doped superconducting diamond. The diamond (black ball) is located between two graphite heaters

Covalent superconductors are superconducting materials where the atoms are linked by covalent bonds. The first such material was boron-doped synthetic diamond grown by the high-pressure high-temperature (HPHT) method.[1] The discovery had no practical importance, but surprised most scientists as superconductivity had not been observed in covalent semiconductors, including diamond and silicon.

## History

[edit]

Magnetic AC susceptibility measured as a function of temperature in diamonds enriched with 12C, 13C, 10B or 11B isotopes. The observation and magnitude of the 12C-13C shift confirms the BCS mechanism of superconductivity in bulk polycrystalline boron-doped diamond.

The priority of many discoveries in science is vigorously disputed (see, e.g., Nobel Prize controversies). Another example, after Sumio Iijima has "discovered" carbon nanotubes in 1991, many scientists have pointed out that carbon nanofibers were actually observed decades earlier. The same could be said about superconductivity in covalent semiconductors. Superconductivity in germanium and silicon-germanium was predicted theoretically as early as in the 1960s.[2][3] Shortly after, superconductivity was experimentally detected in germanium telluride.[4][5] In 1976, superconductivity with Tc = 3.5 K was observed experimentally in germanium implanted with copper ions;[6] it was experimentally demonstrated that amorphization was essential for the superconductivity (in Ge), and the superconductivity was assigned to Ge itself, not copper.

## Diamond

[edit]

Superconductivity in diamond was achieved through heavy p-type doping by boron such that the individual doping atoms started interacting and formed an "impurity band". The superconductivity was of type-II with the critical temperature Tc = 4 K and critical magnetic field Bc = 4 T. Later, Tc ≈ 11 K has been achieved in homoepitaxial CVD films.[7][8]

Regarding the origin of superconductivity in diamond, three alternative theories were suggested: conventional BCS theory based on phonon-mediated pairing, correlated impurity band theory[9] and spin-flip-driven pairing of holes weakly localized in the vicinity of the Fermi level.[10] Experiments on diamonds enriched with 12C, 13C, 10B or 11B isotopes revealed a clear Tc shift, and its magnitude confirms the BCS mechanism of superconductivity in bulk polycrystalline diamond.[11]

## Carbon nanotubes

[edit]

While there have been reports of intrinsic superconductivity in carbon nanotubes,[12][13] many other experiments found no evidence of superconductivity, and the validity of these results remains a subject of debate.[14] Note, however, a crucial difference between nanotubes and diamond: Although nanotubes contain covalently bonded carbon atoms, they are closer in properties to graphite than diamond, and can be metallic without doping. Meanwhile, undoped diamond is an insulator.

## Intercalated graphite

[edit]

Main article: Graphite intercalation compound

Structure of CaC6

When metal atoms are inserted (intercalated) between the graphite planes, several superconductors are created with the following transition temperatures:[15][16]

Material  | CaC6 | Li3Ca2C6 | YbC6 | SrC6 | KC8 | RbC8 | NaC3 | KC3 | LiC3 | NaC2 | LiC2

|
|
|
|
|
|
|
|
|
|
|

Tc (K)  | 11.5  | 11.15  | 6.5  | 1.65  | 0.14  | 0.025  | 2.3–3.8  | 3.0  | <0.35  | 5.0  | 1.9

## Silicon

[edit]

It was suggested[1] that "Si and Ge, which also form in the diamond structure, may similarly exhibit superconductivity under the appropriate conditions", and indeed, discoveries of superconductivity in heavily boron doped Si (Si:B)[17] and SiC:B[18] have quickly followed. Similar to diamond, Si:B is type-II superconductor, but it has much smaller values of Tc = 0.4 K and Bc = 0.4 T. Superconductivity in Si:B was achieved by heavy doping (above 8 at.%), realized through a special non-equilibrium technique of gas immersion laser doping.

## Silicon carbide

[edit]

Superconductivity in SiC was achieved by heavy doping with boron[19] or aluminum.[20] Both the cubic (3C-SiC) and hexagonal (6H-SiC) phases are superconducting and show a very similar Tc of 1.5 K. A crucial difference is however observed for the magnetic field behavior between aluminum and boron doping: SiC:Al is type-II, same as Si:B. On the contrary, SiC:B is type-I. In attempt to explain this difference, it was noted that Si sites are more important than carbon sites for superconductivity in SiC. Whereas boron substitutes carbon in SiC, Al substitutes Si sites. Therefore, Al and B "see" different environment that might explain different properties of SiC:Al and SiC:B.[21]

## Hydrogen sulfide

[edit]

At pressures above 90 GPa (gigapascal), hydrogen sulfide becomes a metallic conductor of electricity. When cooled below a critical temperature its high-pressure phase exhibits superconductivity. The critical temperature increases with pressure, ranging from 23 K at 100 GPa to 150 K at 200 GPa.[22] If hydrogen sulfide is pressurized at higher temperatures, then cooled, the critical temperature reaches 203 K (−70 °C), the highest accepted superconducting critical temperature as of 2015. By substituting a small part of sulfur with phosphorus and using even higher pressures, it has been predicted that it may be possible to raise the critical temperature to above 0 °C (273 K) and achieve room-temperature superconductivity.[23]

## See also

[edit]

* Silicon – chemical element with symbol Si and atomic number 14Pages displaying wikidata descriptions as a fallback
* Silicon carbide – Extremely hard semiconductor
* Synthetic diamond – Diamond created by controlled processes
* Timeline of low-temperature technology

## References

[edit]

1. ^ a b E. A. Ekimov; V. A. Sidorov; E. D. Bauer; N. N. Mel'nik; N. J. Curro; J. D. Thompson; S. M. Stishov (2004). "Superconductivity in diamond". Nature. 428 (6982): 542–545\. arXiv:cond-mat/0404156. Bibcode:2004Natur.428..542E. doi:10.1038/nature02449. PMID 15057827. S2CID 4423950.
L. Boeri, J. Kortus and O. K. Andersen "Three-Dimensional MgB2-Type Superconductivity in Hole-Doped Diamond",
K.-W. Lee and W. E. Pickett "Superconductivity in Boron-Doped Diamond"[permanent dead link],
X. Blase, Ch. Adessi and D. Connetable "Role of the Dopant in the Superconductivity of Diamond"[permanent dead link],
E. Bustarret et al. "Dependence of the Superconducting Transition Temperature on the Doping Level in Single-Crystalline Diamond Films"[permanent dead link] – free download
2. ^ Gurevich V L, Larkin A I and Firsov Yu A (1962). Sov. Phys. Solid State. 4: 185.
3. ^ M. L. Cohen (1964). "The Existence of a Superconducting State in Semiconductors". Rev. Mod. Phys. 36 (1): 240–243\. Bibcode:1964RvMP...36..240C. doi:10.1103/RevModPhys.36.240.
4. ^ R.A. Hein; et al. (1964). "Superconductivity in Germanium Telluride". Phys. Rev. Lett. 12 (12): 320–322\. Bibcode:1964PhRvL..12..320H. doi:10.1103/PhysRevLett.12.320.
5. ^ L. Finegold (1964). "Germanium Telluride: Specific Heat and Superconductivity" (PDF). Phys. Rev. Lett. 13 (7): 233–234\. Bibcode:1964PhRvL..13..233F. doi:10.1103/PhysRevLett.13.233.
6. ^ B. Stritzker; H. Wuhl (1976). "Superconductivity of amorphous Germanium produced by ion implantation". Zeitschrift für Physik B. 24 (4): 367–370\. Bibcode:1976ZPhyB..24..367S. doi:10.1007/BF01351526. S2CID 123326637.
7. ^ Y. Takano; et al. (2007). "Superconducting properties of homoepitaxial CVD diamond". Diam. Relat. Mater. 16 (4–7): 911–914\. Bibcode:2007DRM....16..911T. doi:10.1016/j.diamond.2007.01.027. S2CID 95904362.4–7&rft.pages=911-914&rft.date=2007&rft_id=https://api.semanticscholar.org/CorpusID:95904362#id-name=S2CID&rft_id=info:doi/10.1016/j.diamond.2007.01.027&rft_id=info:bibcode/2007DRM....16..911T&rft.au=Y.+Takano&rfr_id=info:sid/en.wikipedia.org:Covalent+superconductor" class="Z3988">
8. ^ Y. Takano (2006). "Overview". Sci. Technol. Adv. Mater. 7: S1. Bibcode:2006STAdM...7S...1T. doi:10.1016/j.stam.2006.06.003.
9. ^ G. Baskaran (2008). "Impurity band Mott insulators: a new route to high Tc superconductivity". Sci. Technol. Adv. Mater. 9 (4): 044104. Bibcode:2008STAdM...9d4104B. doi:10.1088/1468-6996/9/4/044104. PMC 5099631. PMID 27878017.
10. ^ J. Mares; et al. (2008). "Selected topics related to the transport and superconductivity in boron-doped diamond". Sci. Technol. Adv. Mater. 9 (4): 044101. Bibcode:2008STAdM...9d4101M. doi:10.1088/1468-6996/9/4/044101. PMC 5099628. PMID 27878014.
11. ^ E. A. Ekimov; et al. (2008). "Structure and superconductivity of isotope-enriched boron-doped diamond". Sci. Technol. Adv. Mater. 9 (4): 044210. Bibcode:2008STAdM...9d4210E. doi:10.1088/1468-6996/9/4/044210. PMC 5099641. PMID 27878027.
12. ^ Z.K. Tang; et al. (2001). "Superconductivity in 4 Angstrom Single-Walled Carbon Nanotubes". Science. 292 (5526): 2462–5\. Bibcode:2001Sci...292.2462T. doi:10.1126/science.1060470. PMID 11431560. S2CID 44987798.
13. ^ M. Kociak; et al. (2001). "Superconductivity in Ropes of Single-Walled Carbon Nanotubes". Physical Review Letters. 86 (11): 2416–2419\. arXiv:cond-mat/0010220. Bibcode:2001PhRvL..86.2416K. doi:10.1103/PhysRevLett.86.2416. PMID 11289943. S2CID 15102306.
14. ^ M. Bockrath (2006). "Carbon nanotubes: The weakest link". Nature Physics. 2 (3): 155–156\. Bibcode:2006NatPh...2..155B. doi:10.1038/nphys252. S2CID 125902065.
15. ^ N. Emery; et al. (2008). "Synthesis and superconducting properties of CaC6". Sci. Technol. Adv. Mater. 9 (4): 044102. Bibcode:2008STAdM...9d4102E. doi:10.1088/1468-6996/9/4/044102. PMC 5099629. PMID 27878015.
16. ^ I.T Belash; et al. (1990). "Superconductivity of GIC with Li, Na and K". Synthetic Metals. 34 (1–3): 455–460\. doi:10.1016/0379-6779(89)90424-4.1–3&rft.pages=455-460&rft.date=1990&rft_id=info:doi/10.1016/0379-6779(89)90424-4&rft.au=I.T+Belash&rfr_id=info:sid/en.wikipedia.org:Covalent+superconductor" class="Z3988">
17. ^ E. Bustarret; et al. (2006). "Superconductivity in doped cubic silicon". Nature. 444 (7118): 465–8\. Bibcode:2006Natur.444..465B. doi:10.1038/nature05340. PMID 17122852. S2CID 4383370.
18. ^ Zhi-An Ren; et al. (2007). "Superconductivity in Boron-doped SiC". J. Phys. Soc. Jpn. 76 (2): 103710. Bibcode:2007JPSJ...76b3710M. doi:10.1143/JPSJ.76.023710. hdl:2433/136766.
19. ^ M. Kriener; et al. (2008). "Superconductivity in heavily boron-doped silicon carbide". Sci. Technol. Adv. Mater. 9 (4): 044205. arXiv:0810.0056. Bibcode:2008STAdM...9d4205K. doi:10.1088/1468-6996/9/4/044205. PMC 5099636. PMID 27878022.
20. ^ T. Muranaka; et al. (2008). "Superconductivity in carrier-doped silicon carbide". Sci. Technol. Adv. Mater. 9 (4): 044204. Bibcode:2008STAdM...9d4204M. doi:10.1088/1468-6996/9/4/044204. PMC 5099635. PMID 27878021.
21. ^ Y. Yanase; N. Yorozu (2008). "Superconductivity in compensated and uncompensated semiconductors". Sci. Technol. Adv. Mater. 9 (4): 044201. Bibcode:2008STAdM...9d4201Y. doi:10.1088/1468-6996/9/4/044201. PMC 5099632. PMID 27878018.
22. ^ A. P. Drozdov; et al. (2015). "Conventional superconductivity at 203 kelvin at high pressures in the sulfur hydride system". Nature. 525 (7567): 73–76\. arXiv:1506.08190. Bibcode:2015Natur.525...73D. doi:10.1038/nature14964. PMID 26280333. S2CID 118573189.
23. ^ Cartlidge, Edwin (18 August 2015). "Superconductivity record sparks wave of follow-up physics". Nature. 524 (7565): 277. Bibcode:2015Natur.524..277C. doi:10.1038/nature.2015.18191. PMID 26289188.

## External links

[edit]

* International Workshop on superconductivity in Diamond and Related Materials 2005
* International Workshop on Superconductivity in Diamond and Related Materials 2008
* New Diamond and Frontier Carbon Technology Volume 17, No.1 Special Issue on Superconductivity in CVD Diamond
* Some papers on superconducting diamond

* v
* t
* e

Superconductivity

Theories|

* BCS
* Bean's critical state
* Ginzburg–Landau
* Kohn–Luttinger
* London
* Matthias
* Mattis–Bardeen
* RVB
* WHH

Characteristic parameters|

* coherence length
* critical field
* London penetration depth
* Silsbee current

Phenomena|

* Abrikosov vortices
* Andreev reflection
* Cooper pairs
* flux pinning
* flux pumping
* Josephson effect
* Little–Parks effect
* Meissner effect
* Homes's law
* persistent currents
* proximity effect
* reentrance
* SU(2) color
* supercurrents
* superdiamagnetism
* superstripes

Classification|

| By magnetic response|

* Types
* I
* II
* 1.5
* ferromagnetic

|

By explanation|

* conventional
* unconventional
* topological

By critical temperature|

* low temperature
* high temperature
* room temperature

By composition|

* covalent
* cuprates
* heavy fermion
* iron-based
* oxypnictides
* organic

Technological applications|

* cryotron
* electromagnets
* MRI
* NMR
* quantum computing
* Rutherford cable
* SQUID
* wires
* SCMaglev

List of superconductors|

* bilayer graphene
* BSCCO
* LBCO
* MgB2
* NbSn
* NbTi
* TBCCO
* YBCO
* more...

*[v]: View this template
*[t]: Discuss this template
*[e]: Edit this template